Dottorato di ricerca in
Scienza e Tecnologia dei Materiali Innovativi
Ciclo XXVII (2012-2014)
Synthesis and characterization of novel nanosystems for biomedical applications
Chiar.mo Prof. Enrico Dalcanale Tutor:
Chiar.ma Prof. Franca Bigi
Dottoranda: Elena Bedogni
A mia mamma e mio nonno
Nanomedicine ... 1
Nanoparticles ... 3
Nanowires ... 16
Porphyrins and photodynamic therapy ... 19
BioNiMed ... 25
References ... 26
Synthesis and characterization of superparamagnetic Fe3O4 nanoparticles Introduction ... 30
Results and Discussion ... 32
Experimental Section ... 45
References ... 49
Synthesis of a nanosystem composed by Fe3O4 nanoparticles bound to SiC/SiOx nanowires Introduction ... 52
Results and Discussion ... 59
Experimental Section ... 65
References ... 68
Synthesis and characterization of various porphyrins Introduction ... 72
Results and Discussion ... 76
Experimental Section ... 93
References ... 102
Introduction ... 106
Results and Discussion ... 108
Experimental Section ... 127
References ... 134
Synthesis of Fe3O4 –mSiO2 nanoparticles Introduction ... 137
Results and Discussion ... 139
Experimental Section ... 155
References ... 158
Conclusions 159 Future works 163 Acknowledgements
Nanoscience and nanotechnology are now well established scientific and engineering disciplines. This is evidenced by the investments of government funding programs specifically targeting nano-research and development, the proliferation of research journals devoted to nano and the massive investment by worldwide research institutions in nanotechnology facilities, infrastructure and personnel.
Figure 1 . Correlation between visual objects and micro- and nano-compounds. Nano is the prefix for the unit that are 10-9 m in size. Nanometer is a billionth of a meter (a
Nanotechnology requires the ability to understand and to precisely manipulate and control nanoscale materials in a useful way.
Nanomedicine is emerging as one of the most important sub-disciplines under the nanotechnology umbrella.
Nanomedicine was definite (by the European Science Foundation, ESF) as “the science and technology of diagnostic treating and preventing disease and traumatic injury, of relieving pain, and of preserving and improving human health, using molecular tools and molecular knowledge of the human body”. Nanomedicine is defined as the application of nanometer technologies in medical areas (from biomedical imaging to drug delivery and therapeutics). This is a new and fast expanding medical field. The overall goal of nanomedicine is the same as it is for traditional medicine: early and accurate diagnosis, effective treatments that are free of side effects, and non-invasive evaluation of the efficacy of the treatment. Nanotechnology is a very broad interdisciplinary research field that involves various areas of science and chemistry. Physics and engineering properties of nanomaterial can change completely if you compare the nanosystem with bulk phenomena. Some of these nanosystems are already appearing in the market place or as clinical trials.
In the world and also in Italy, the interest in nanodevices and nanosystems for biomedical applications is growing rapidly.
Nanoparticles are characterized by an high surface to volume ratio, and the large percentage of surface atoms compared with bulk materials are the results of the small size. Due to their size, the nanodevices (like nanoparticles) can possess properties useful in biomedical field, being in the same range of dimension like nucleus, protein and so on.
There are numerous journals publishing papers dealing with nanoparticles for various applications and many of them are specifically devoted to nanomaterials. Researchers at Rice University have demonstrated that cerium oxide nanoparticles act as an antioxidant to remove oxygen free radicals that are present in a patient's bloodstream following a traumatic injury.3 The nanoparticles absorb the oxygen free radicals and then release the oxygen in a less dangerous state, leaving free the nanoparticles to absorb more free radicals.
Another example is reported by MIT, where nanoparticles are used to deliver vaccine. The nanoparticles protect the vaccine, allowing the vaccine time to trigger a stronger immune response.4 Other groups are developing ways to use carbon nanoparticles called nano-diamonds in medical applications.5 For example, nano-diamonds with attached protein molecules can be used to increase bone growth around dental or joint implants. Some other researchers are testing the use of chemotherapy drugs attached to nanoparticles to destroy the cancer cells. 6
In according with the chemical composition, the nanoparticles can have powerful properties like imaging for in vivo analysis or in vitro test.
The presence of receptors or smart molecules makes possible to use this nanosystems for obtaining diagnostic responses as well as the presence of specific drugs, makes possible to apply the therapy in a local and specific area. In recent years a new generation of very efficient nanoparticles allowed to create multifunctional systems that have bonded together different functional groups. For in vitro and in vivo
applications in biomedical field, nanoparticles have to possess the following features:
• small overall size,
• high surface area for a specific functionalization,
• high colloidal stability,
• capacity to cross the cell walls in order to enter the cells and then perform their function
• non toxicity,
• non immunogenicity,
• capable to stay in solution for long time.
Therefore, we can conclude that for biomedical application the aim is to obtain multifunctional nanoparticles with a narrow size distribution, non-aggregated and stable for long time in biological media.
Nanoparticles can have different applications7 according with the crystal structure, the shell composition, the shape and size. The performance as drug delivery system has been improved enormously because of the development of controlled release of drugs under some specific stimulation (changing pH, light, temperature, presence of specific substances…).
The development of targeted delivery possible to release the drug just inside the specific area of the body). In order to further improve the drug delivery process, some crucial properties of the free drugs such as solubility, in vivo stability, pharmacokinetic, and bio distribution must be considered. The overall efficacy can be improved by using suitable nanoparticles carrying drug with increasing selectivity toward the targeted tissue.
Different types of molecular imaging techniques, such as optical imaging (OI), magnetic resonance imaging (MRI), ultrasound imaging, positron emission tomography (PET), and others are used for the imaging of both in vivo and in vitro biological specimens. However, optical and magnetic resonance imaging techniques are the most acceptable because they utilize the inherent luminescent and magnetic properties of nanoparticles. Some other applications are in sensor field.
Sensor is a device that measure a physical quantity and converts it into an analog or digital signal that can be read by an instrument. In in vivo applications, nanoparticles are also used like a sensor for the detection of damaged cells, DNA, RNA, glucose, cholesterol …
A magnetic material coated with a fluorescence material can also be used as sensor. Here the fluorescence dye tracks the particle location, whereas the magnetic core serves to transfer heat at that position via magnetic excitation.
Nanoparticles coated with a functional material such as a noble metal, semiconductor, or appropriate oxide have increased the physical properties (optical, catalytic activity, electrical, magnetic and thermal) of the combine particles compared with the pure core particles.
Among the nanoparticles, superparamagnetic ones properties have been intensively developed not only for their fundamental scientific interest
but also for many technological applications, such as target in drug delivery8, as contrast agent in magnetic resonance imaging (MRI)9 and also as magnetic inks for jet printing10. The control of the size and dispersal is very important since the properties of the nanocrystals strongly depend upon the dimension of the nanoparticles.11 Superparamagnetic iron oxide nanoparticles depending on the surface modification can be used for numerous in vivo applications, such as MRI contrast enhancement, tissue repair, detoxification of biological fluid, immunoassay, cell separation, hyperthermia and drug delivery.
All these techniques require magnetic nanoparticles with large magnetization value, size smaller than 100 nm and narrow size distribution. These applications also need peculiar surface coating of the magnetic particles, which as to be non toxic and biocompatible, allowing also a targetable delivery with particle localization in a specific area. Magnetic nanoparticles binding drugs, proteins, enzymes, can be directed toward an organ, tissue, or tumor using an external magnetic field.
Another sector of application is the environmental field. Besides treatment of exhausts mono particulate catalysts are employed in waste water treatment. For example Pd-Fe3O4 composite catalyst was used for environmentally friendly treatment of AOX polluted substance (AOX: absorbable organically bound halogens). In China Feng et al.12 are studying the adsorption of ions in exhaust water using magnetic nanoparticles coated with specific functional groups. Among the various superparamagnetic nanoparticles, magnetite displays the best magnetic properties.
In particular, the project developed in the present work is combine the hyperthermia properties of Fe3O4 nanoparticles with the photodynamic properties of a photosensitizer for a bimodal treatment of cancer.
Aiming to prepare a single nanosystem able to display both properties for deep cancer treatment, the functionalization of cubic SiC/SiO2
nanowires with Fe3O4 nanoparticles and with porphyrins was studied.
There are different ways to synthesize Fe3O4 nanoparticles. The first one was the co-precipitation method described by Massart et al.13 , that
starts from salts of iron (III) and iron (II) in a stoichiometric ratio and heated under basic condition. The nanoparticles obtained by this method are not well stabilized, since the stabilization come only from the OH ion on the surface.
Indeed usually they form aggregates (Fig. 2) that for biomedical application are unwanted.
Other two synthetic routes are microwave and thermal decomposition method. The last one is the method that I used, and it will be described in details in the second chapter.
Microwave method is a new and efficient method that starts from the same precursors, such as Fe(ac)x or Fe(acac)x employed in thermal decomposition. Being very energetic conditions, the reaction takes a very short time. The critical point could be the very fast reaction which often determines a non-good crystallinity.
Magnetite has the following composition Fe3O4 and has an inverse spinel crystal structure. The 32 O2− ions have a cubic close packing (ccp) with an ABCABC stacking. The anions packing gives rise to two diﬀerent interstitial sites: tetragonal and octahedral sites. The spatial crystal group is Fd3m and the unit cell dimension is 0.8369 Å (Fig. 3).
Figure 2. TEM picture shows the magnetic nanoparticles obtained by co- precipitation method.
Figure 3. Magnetite crystal structure: ccp of oxygen anions (white balls) with Fe2+
Fe3+ (red balls).
The tetrahedral sites are occupied by Fe3+ cations while the octahedral are occupied by both Fe2+ and Fe3+ randomly distributed. The inverse spinel structure can be written as Y [XY]O4 where X = Fe2+ Y = Fe3+
and the brackets indicate octahedral sites.
Below the Curie temperature TC= 850 K, magnetite is ferromagnetic material
This material is also characterized by a structural transition (Verwey transition) as a function of temperature. The ﬁrst observation of this phase transition was observed by Renger in 1913 on a synthetic polycrystal, measuring the initial susceptibility as a function of temperature. The ﬁrst electric measurements as a function of temperature, in which the evidence of a change in resistivity was observed, were done by Okamura14 and Verwey15. They observed a variation of resistivity by about a factor of 100 at the critical temperature TV ≈ 125K (Verwey transition temperature). At the beginning no structural transition was identiﬁed by XRD and only later the crystal structure was solved16. Verwey explained the variation of all the structural parameters considering that
1. above TV, the Fe2+ and Fe3+ ions are randomly distributed over the B-sites, permitting relatively easy valance exchange by means of thermally activated fast electron hopping
Fe2+ −e ⇌ Fe3+
2. below the critical temperature, there is a reduction of the crystal symmetry from cubic to tetragonal and the charges order in a way that successive, a/4-spaced (100) lattice planes would be occupied, alternatively, by ferric and ferrous ions.
In this way, above the Verwey transitions the electronic conduction is described by a thermally activated hopping process between the ferrous and ferric ions in the octahedral lattice sites, and their random distribution gives rise to an isotropic conductivity17.
Superparamagnetism of nanostructured material
The magnetic properties of nanomaterials strongly depend on the size as show in figure 4.
Figure 4. (a) Coercivity as a function of the particle sizes and (b) typical hysteresis loop shape for systems showing superparamagnetic (red), paramagnetic (green) and ferromagnetic (blue) properties.
For our purpose, we need nanoparticles in the superparamagnetic state.
Superparamagnetism arises only in systems constituted by very small nanoparticle sizes, smaller than 20 nm in the case of Fe3O4. In this regime, the magnetic moments are randomly distributed and can randomly flip their direction under the influence of temperature. The
typical time between two flips is called the Néel relaxation time. In the absence of external magnetic field, when the time used to measure the magnetization of the nanoparticles is much longer than the Néel relaxation time, their magnetization appears to be in average zero. In this state, an external magnetic field is able to magnetize the nanoparticles, similarly to a paramagnet. However, their magnetic susceptibility is much larger than the one of paramagnets. Only below a critical temperature called blocking temperature TB, the magnetic moments are blocked, and the thermal energy becomes unable to affect the system. A magnetic order establishes giving rise to ferromagnetic properties.
The equation that describes the relation between magnetization and magnetic field is:
! = !" ∙ !
where ! is the magnetization, ! the magnetic field and !" the magnetic susceptibility, a positive number which increases decreasing the temperature.
Another relation is:
! =! − !!!
! = !!!! 1 + !" = !!
Where µ is the magnetic permeability.
Superparamagnetic materials are characterized by two important properties:
• high saturation magnetization MS
• no remanence MR (value of the magnetization in sero applied magnetic field).
The superparamagnetic property depends from the size of nanoparticles. This property is manifested in magnetite nanoparticles only under the limit of 20 nm. Over this critical size, the magnetization curves show an hysteresis, with a non-zero remanence and coercivity . On the other hand, for size much lower than this critical size the magnetization becomes too low and in some case it is almost impossible to catch up. In our case the goal is to achieve a high value for saturation magnetization remaining below the limit imposed by superparamagnetism.
One of the most interesting application of superparamagnetic nanoparticles (MNPs) is the magnetic hyperthermia. MNPs are mediator of heat transfer when a radio-frequency magnetic field is applied. When an alternate magnetic field is applied many phenomena occur:
(i) the spins rotate inside the nanoparticle, and this internal friction generates heat which is transferred outside by way of thermal conductivity,
(ii) because of the coupling between the magnetic moment and the particle, the particle itself starts to rotate with respect to the matrix, generating a deformation around the particle and heat is produced as a consequence of viscous dissipation..
The local tissue temperature has to be higher than 42°C but lower than 47°C for almost 30 min., to destroy cancer cells, while the healthy cells are less affected. The product of applied field and frequency has to be lower than 4.85 108 A/ms.18 These parameters have to be controlled because of peripheral and skeletal muscles, possible cardiac stimulation and arrhythmia and non-specific inductive heating of tissue. Therefore frequencies and amplitudes must be f = 0.05-1.2 MHz and H=0-15 kAm-1.19 The nanoparticles can be directly injected in tumor or can be injected through intravascular administration or antibody targeting.
This method isn’t efficient enough when applied alone20, even if for certain types of cancer, it is more suitable than the conventional treatments of radiotherapy and chemotherapy; in particular when the tumor is located close to vital organs or is drug resistant. Sometimes it is used together with chemotherapy, in fact below 42°C, it doesn’t directly cause cell death but can increase the effect of certain chemotherapy drugs that are more active at higher temperatures, and in this way a lower dose is required.
Radiotherapy can also be used with hyperthermia21. The ability of a magnetic material to be a hyperthermic mediator depends on many different parameters and the mechanism of heating is not well understood it can be due to losses in a hysteresis cycle, susceptibility loss, or frictional heating due to particle rotation in a liquid environment.
When a magnetic moment is exposed to a field there exists a magneto static energy and in order to reduce its magneto static energy it rotates to align with the field. If low field strength is applied at a high frequency the moment can’t follow the field and heat is generated due to this phase lag and also to frictional effects.
If we consider multi domains MNPs, the effects of heat transfer are related to the mechanism of hysteresis loop, as well movement. The amount of heat generated per unit volume PFM is given by frequency of multiplied by area of hysteresis loop:
!!" = !!! ! !"
For ferromagnetic particles well above the super-paramagnetic size limit the !!" can be approximately determined from quasi static measurements of the hysteresis loop. The orientation and growth of spontaneously magnetized domains within a given ferromagnetic particle depends on both microstructural features such as vacancies, impurities or grain boundaries, and intrinsic features such a magneto- crystalline-anisotropy as well as the shape and size of particles. If we consider instead single domain nanoparticles near to super- paramagnetic size we can identify two mechanisms: hysteresis loses, relaxation of magnetization when an alternating field is applied leads to a frequency dependence of hysteresis loss. The remanence and the coercivity increase at high sweep-rate, increasing loop squarenes 222324 and the hysteresis losses are proportional to the square of the frequency. At high frequency, in fact, some nanoparticles are not in super-paramagnetic state. Therefore we can conclude that frequency of the alternating applied field is an important parameter in controlling the amount of heat produced from hysteresis losses. Another mechanism of
release of heat is the physically rotation of particles in order to align their moments with an applied field. It is called Brownian relaxation and depends on hydrodynamic volume of nanoparticles, VH, on the solvent viscosity η and on temperature T:
!! = !3!!!!
Where' !=KVM/(kT). The other mechanism of relaxation of magnetization is the Nèel relaxation that is due to the thermal fluctuation of magnetization at a given temperature. 25
!" = ! !
For both relaxation times there is a dependence from volume and therefore from of the MNPs size. The particles suspended in a colloidal Ferrofluid have a reduced heating when Brownian relaxation is prevented, but when injected into a tumor the ability of the particles to move freely will be reduced and Brownian losses are unable to contribute to the heating. For non-interacting magnetic nanoparticles in a single domain state, we can describe the power dissipation through the model of Rosensweig). An optimum particle size exists at which corresponds the maximum power heating, independently from the applied field intensity. The critical size strongly depends on the material of nanoparticles, being due mainly to the anisotropy constant, an intrinsic property. Another mechanism of heating is the presence of eddy currents. The electrical conductivity of the particles induces eddy currents at the surface of the particles when an alternating field is applied, producing heat due to the resistance of the material. . The eddy currents have been shown to be negligible for small particles (less the 100 nm in diameter) if the frequency of the alternating field is also less the 10 GHz.
Other characteristics influence the heat rate, i.e. MNPs size distribution, the surface functionalization26,27,28,29, the anisotropy and the
interactions, the ferrofluid parameters as well as the concentration of nanoparticles in solution and the solvent properties.30
The heating capacity of a magnetic material is quantified through the specific absorption power rate (SAR), defined as the amount of energy converted into heat per time and per mass. The following equation describe SAR:
!"# = !"!"
where Cs is the sample heat capacity (that is specific for each sample).
In the last decade nanowires became really important in different fields, such as mechanics, electronics and in nanomedicine. Several nanosystem are being studied. Such as carbon nanotubes (single-walled and multi-walled). Metal nanowires (e.g. based on gold, iron and silver), semiconducting nanowires (e.g. silicon, GaN and other III-V nanowires), and oxide nanowires (e.g. ZnO, SiO2, and TiO2). Further, SiC nanowires are being studied as neuronal probes for their cytocompatibility and better performances respect to other materials.31 During my PhD thesis work I developed some methods to functionalize core-shell SiC/SiOx nanowires, supplied by the IMEM-CNR Institute of Parma, where they were grown and characterized. These nanowires are composed by core of cubic silicon carbide and shell of silica, as well evidenced in Figure 5.
The technique employed for the preparation of the nanowires is called chemical vapour deposition (CVD) and consists in the growth of the nanowires on a silicon substrate, without removing the native oxide and in the presence of metal catalysts. In this technique, the substrate is pre- treated with an iron salt, then exposed to a stream of CO mixed with N2
and Ar as carrier gas. The growth of the nanowires is catalyzed by the iron and occurs at temperatures between 1050-1100 °C. During this time, the carbon monoxide diffuses across silica and at the interface between SiO2 and Si. Where the following carbothermic reaction between CO and Si occurs:
4 CO (g) + 6 Si (s) = 4 SiC(s) + 2 SiO2
In agreement with the preferential mechanism of nucleation at the interface vapor-liquid (VLS), the formation of a dense forest of nanowires SiC/SiO2 can be observed. The nanowires obtained were characterized by various analytical techniques, including transmission electron microscope, cathodoluminescence, X-Ray and Raman spectroscopy. The results confirm that the nanowires actually have a structure “core-shell”, with a core of about 15-20 nm and a coating of approximately equal thickness, for total diameter of about 60 nm.
In our project, I developed methods of functionalization, , of core-shell nanowires, exploiting different materials. The system produced at the IMEM-CNR of Parma is composed by a core of silicon carbide SiC and a shell of silica SiO2 as reported in Figure 5.
As reported by Fabbri et al.32, SiC is biocompatible33,34 and can be of great interest for biomedical applications, in particular if functionalized with specific organic macromolecules like porphyrins (described later).
This core-shell inorganic-organic system can create an active anticancer device when excited by energetic X-Ray radiation. The energy associated to this radiation activates the green emission of SiC in its cubic phase, which in turn determines the production by phorphyrins of the singlet oxygen, the best cytotoxic agent produced in photodynamic therapy (see next paragraph)35,36.
Fabbri et al.37 observed that the silica shell improved the emission of the SiC core.
Figure 5. Zero-loss image of core-shell nanowire by TEM
They proposed a model to explain why the presence of the silicon dioxide shell increases the radiative recombination in the silicon carbide core. A type I band alignment of 3C-SiC and SiO2 can be hypothesized. The conduction and valence band offsets have been experimentally found in the case of bulk material29 and they are equal to ΔEc= 3.6 eV and ΔEv= 2.9 eV, respectively as reported in Figure 6.
The carriers generate by the electron beam in the shell diffuse into the core, where it can recombine according to the allowed transitions in
3C-SiC. No effects are observed in the energy transfer from the shell to the core.
Figure 6. Sketch of the type I band alignment between 3C-SiC and SiO2. Fabbri et al.
The diffusion of the carriers could be considered as an energy transfer from the shell to the core (it was the first time that this effect was observed in NWs).
In this type of NWs the shell is beneficial in enhancing the luminescence intensity of the crystalline core, preferentially the SiC NBE radiative recombination. In the model’s figure (Figure 6) the quantum confinement effect depends from the size core of SiC.
1.4 Porphyrins and photodynamic therapy
Porphyrins and related macrocycles provide an extremely versatile synthetic base for a variety of material applications. The exploration of metal porphyrins assemblies as building blocks for tailored material properties has grown rapidly during the past decade. The nonlinear optical properties of these materials are of special interest, also for potential applications in optical communications, data storage, and electro-optical signal processing. Porphyrins are extensively employed as photosensitizers in photodynamic therapy for the treatment of superficial tumors, and new structures of porphyrin are being proposed to improve their properties and to use more penetrating radiation.
During my thesis I synthesize porphyrins as photosensitizers and prepared new hybrid nanosystems conjugated with porphyrins for possible photodynamic therapy.
It’s due a briefly explanation of the activity of this type of molecules.
Singlet oxygen generated by the photosensitizer from molecular triplet oxygen is the principal toxic species formed during PDT, although the extent to which these species are responsible for the photodynamic effect is under debate. Nevertheless, the generation of singlet oxygen is extremely crucial to the success of PDT, and one of the first tests performed on new PDT drugs is to probe their ability for singlet oxygen generation.38,39 Figure 7 shows the modified Jablonski’s diagram for a typical photosensitizer.
Figure 7. Modified Jablonski diagram for a typical photosensitizer
Of particular importance with regard to PDT is that the excited photosensitizer can undergo the non-radiative process of inter-system crossing. This is a spin-forbidden process which requires spin inversion, thereby converting the photosensitizer to a triplet state.
Any “forbidden” pathway is less likely than an “allowed” process, but a good photosensitizer undergoes the “forbidden” ISC pathway with very high efficiency. The molecule can relax from the triplet via at least two pathway: radioactively by fluorescence, and non-radioactively by spin exchange with another triplet state molecule.
Fluorescence involves a spin-inversion which is also spin-forbidden, and imposes a relatively long lifetime of the triplet state, on the microsecond time scale. This allows the interaction between molecules close to the excited photosensitizer. One interaction is spin exchange (also corresponding to energy transfer) with triplet oxygen, which generates the highly reactive singlet oxygen species, one of the most
reactive species having a lifetime in water of roughly four microseconds. It undergoes several reactions with biological substrates such as oxidation or cycloaddition or a kind of reactions that are disruptive to biological processes. An important photophysical property is represented by the efficiency of transferring the energy of the absorbed light from the triplet state of the photosensitizer to the triplet oxygen with the consequent generation of singlet oxygen, defined also as the singlet oxygen quantum yield.
There is only an indirect evidence for the production of singlet oxygen in a biological system since the lifetime of singlet oxygen is so short that cannot be observe directly. The application of light is of primary importance to the efficacy of PDT. Like the number and the types of photosensitizer compounds have been increasing over recent years, also the variety of light sources were considerably increased.
The basis of the structure of porphyrins skeleton is formed by four pyrroles linked with four methine bridges (Fig. 8).
Figure 8. Porphyrin ring
Porphyrins (from the Greek means purple, scarlet) are based on 16 – atom rings containing four nitrogen atoms. They are macro cycles that contain only sp2-hybridized bridging meso carbon atoms within their framework. The structure is fully aromatic, contains 18 π-electrons.
They are in a perfect size to bind nearly all metal ions.40
By substitution of hydrogens in the meso-position with some substituents, complex porphyrins can be obtained. Depending on the synthesis, the substituents in the meso-position can either be the same or different. The basic porphyrin skeleton can be synthesized by several routes based on condensation reactions between aldehydes, pyrroles,
dipyrromethanes or similar precursor under acidic conditions and subsequent oxidation. Symmetric porphyrins are more easily synthetized than asymmetrical ones. Their synthesis is based on a condensation of pyrrol and aldehyde with different reaction conditions (like Adler-Longo conditions).41 The first prepared symmetrical porphyrin had four phenyl substituents in meso-positions.
On the other hand, the asymmetrical porphyrins are much less synthetically accessible. Their preparation is based on various approaches (like a Adler-Longo conditions or 2+2 approach, 3+1 approach and so on). The first time that the activity of porphyrins was found to be useful in the photodynamic therapy was in 1913, when Meyer Betz injected himself with 200 mg of hematoporphyrin and registered no ill effects until he exposed himself to sunlight, whereupon for several months he suffered extreme swelling. The most recent photoactive based drug therapy utilizes phorphyrin-based chromophores in combination with visible light. Phototherapy was dormant for several decades, although the idea that light could be a therapeutic modality was well explored. Photodynamic therapy (PDT), a new treatment modality, involves administration of a tumor-localizing photosensitizing agent (PS) followed by activations of the agent by light of a specific wavelength. This result in a sequence of photochemical and photobiological processes that cause irreversible photodamage in tumor tissues. The hallmark of PDT is intracellular oxidative stress mediated by reactive oxygen species. In order to achieve the most efficient photosensitizer effect in tumor cells, two are the possibilities, the sensitizer must enter the cells or it has to become closely associated with the subcellular structure. Photosensitizer may enter cells either directly through the plasma membrane or by endocytosis. Uptake over the plasma membrane may occur by simple or facilitated diffusion or by an active transport mechanism. Cancer cells, in common with other rapidly proliferating cells, may have an increased requirement of cholesterol for membrane biosynthesis. They may therefore upregulate the expression of the low-density lipoprotein (LDL) receptor. It is know that lipoproteins are major carriers of
lipophilic porphyrins in the bloodstream and may therefore be a means of entry of these compounds into cells.
A decreased intra tumor pH may affect the ionization of porphyrin species, reducing in this way the activity of PDT.
Tumors contain increased numbers of lipid bodies and particularly neutral lipid droplets; in addition their cell membranes may be more hydrophobic than those of normal cells.
A combination of “leaky” tumor vasculature and reduced lymphatic drainage might encourage the build-up of porphyrins in the interstitial space. In tumors cells can increase capabilities for phagocytosis or pinocytosis, this effect can became dangerous for porphyrin aggregates and nanosystem.
The porphyrin can have different R-groups (Figure 8). In my case I worked with meso porphyrin and asymmetric ones in order to examine different rings and different symmetry.
Figure 10 I explains the steps of photodynamic therapy starting from the transport of sensitizer inside the human body, then the distribution inside the specific tissue, and the differential clearance tissue. After that there is the excitation to the photosensitizer and consequently the chemical and biological damage with cells and tissue necrosis.
The aim of my thesis is to synthetize nanosystems for biomedical applications, in particular for anticancer therapy.
The idea and research funding come from a project called BioNiMed, written by Dott. G. Salviati of the IMEM-CNR Parma. The final aim is the synthesis of nanosystems constitued by core shell SiC@SiOx
nanowires decorated with porphyrins and Fe3O4 nanoparticles and. The final system, combining the properties of the MNPs and porphyrins, could be suitable both for the photodynamic and the hyperthermia therapy.
The aim of my PhD thesis was the preparation and characterization of hybrid nanosystems for application in nanomedicine, with particular interest to the possible anticancer therapies. The anticancer effect can be induce by the magnetic hyperthermia therapy using magnetite nanoparticles and the photodynamic therapy induced by a irradiation of a specific system by X-rays. For increasing the efficiency of the hyperthermia therapy, we developed also core shell nanoparticles, able to encapsulate and release drug thanks to the mesoporous shell. This part of the work was done in Functional Nano Meterial (FNM) group in Stockholm (Sweden) under the supervision of Professor M. Toprak and Professor M. Mohamed at KTH, Royal Institute of Technology.
Thanks to the collaboration with Mutti’s and Petronini’s group at University of Parma, the systems were also characterized from the biological point of view, we perform in vitro study for the evaluation of the activity and biocompatibility of the system.
2 Charles R M., Welcome to Nanomedicine, Nanomedicine 1 (1), 5- 5(2006)
3 S. S. Lee, W. Song, M Cho, H. L. Puppala, P. Nguyen, H. Zhu, L.
Segatori, and V. L. Colvin ACS Nano, 2013, 7 (11), 9693–9703
4 D. J. Irvine, M. A. Swartz, and G. L. Szeto; Nat Mater.; 12(11): 978–
5 L. Moore, M. Gatica,H. Kim, E. Osawa,and D. Ho; J Dent Res.;
92(11): 976–981. (2013)
6 I. Rivkin, K. Cohen, J. Koffler, D. Melikhov, D. Peer, R. Margalit.
Biomaterials, 31 (27): 7106 (2010)
7 C. R. Ghosh , S. Paria Chem. Rev., 112, 2373-2433 (2012)
8 T.K Jain, M.A. Morales, S. F. Cheng, S. Bounnak, Appl. Phys. Lett., 81, 2211 (2002); I. Chourpa, L. Douziech-Eyrolles, J.F. Ngaboni- Okassa. S. Cohen-Jonathan, M. Source, H. Marchais, P. Dubois, Analyst 130(10), 1395 (2005)
9 J. W. Bultè, Methods Mol. Med. 124, 419 (2006), M. Modo, J. W.
Bultè, Mol. Imaging 4 (3), 143 (2005)
10 S. W. Charles, J. Popplewell, J. Endeavour, 6, 153 (1982)
11 S. Laurent, D. Forge, M. Port A. Roch, C. Robic, L. Vander Elst, and R. N. Muller Chem. Rev., 108, 2064-2110, (2008)
12 L Feng, M Cao, X Ma, Y. Zhu, C. Hu; Journal of Hazardous materials 217-218 439-446, (2012)
13 Massart, R. J., “Preparation of magnetite nanoparticles”, IEEE Trans Magn., 17, 11247-11250 (1981)
Bee, A., Massart, R., Neveu, S., J. Magn. Magn. Mater., 149, 6-9 (1995)
14 B.S. Ellefson, N.W: Taylor J.Chem. Phys., 2:58, (1934).
15 E.J.W. Verwey. Nature, 144:327, (1939)
16 W.H. Bragg. Nature, 95:561, (1915)
17 F. Walz. J. Phys.: Condens. Matter, 14:R285, (2002)
18 W.J. Atkinson, I. A. Brezovich, D. P. Charaborty IEEE Trans.
Biomed. Eng., 31:70, (1984)
19 Q. A. Pankhurst, J. Connolly, S. K. Jones, and J. Dobson. J. Physic.
D: Appl. Phys., 36:R167, (2003)
20 B. Hildebrandt, P. Wust, O. Ahlens Crit. Rew. Oncol. Hematol., 43:33, (2002)
21K. Maier-Huff et al. Int. J. Neuroncol. , 241;317, (2011)
22 R. W. Chantrell, G. N. Coverdale, and K. O’Grady J. Phys. D: Appl.
Phys., 21:1469, (1988)
23 M. El-Hilo, A. M. de Writte, K. O'Grady, and R. W. Chantrell,. J.
Magn. Magn. Mater., 117:307, (1992)
24 A. M. de Witte, M. El-Hilo, K. O'Grady, R. W. Chantrell, J. Magn.
Mater., 120: 184, (1993)
25 Nedelcu G. Mangetic nanoparticles impact on tumoral cells in the treat- ment by magnetic fluid hyperthermia. Digest Journal of Nanomaterials and Biostructures Vol. 3, No. 3, (2008)
26 R. Hergt; S. Dutz, M. Roder J. Phys.: Condens. Matter, 20:385214, (2008)
27 G. Goya, Jr. E Lima, A.D. Arelaro, T. Torres, H. R. Rechenberg, L.
Rossi, et all EEE Trans. On Mag., 44:4444, (2008)
28 M. A. Gonzalez-Fernandez, T.E. Torres, M. Andre ´s-Verge ´s, R.
Costo, P. de la Presa, C.J. Serna, et al. J. Sol. State Chem., 182:2779, (2009)
29 G. F. Goya, R. Fernandez-Pacheco , M. Arruebo , N. Cassinelli and M. R. Ibarra, J. Magn. Magn. Mater., 316, 132 -135 (2007)
30 E. Lima Jr, E. De Biasi, R. D. Zysler, M. V. Mansilla, M. L. Mojica- Pisciotti, T. E. Torres, M. P. Calatayud , C. Marquina • M. R. Ibarra • G.F. Goya, J Nanopart Res 16:2791 (2014)
31 C.L. Frewin, C. Locke, S.E. Saddow,E:J: Weeber; Silicon Carbide Biotechnology, Inc. E., Ed., 209-256 (2012)
32 F. Fabbri, F. Rossi, G. Attolini, G. Salviati, S. Iannotta, L. Aversa, R.
Verucchi, M. Nardi, N.Fukata, B. Dierre and Takashi Sekiguchi, Nanotechnology 21 345702 (2010)
33G. Colletti, M J Jaroszeski, A. Pallaoro, A.M. Hoff, S. Iannotta and S.
E. Saddow, Proc. 29th Annu. Int. Conf. IEEE EMBS vol 5849 (2007)
34 G. Cicero, A. Catellani and G. Galli. 93 016102 Phys. Rev.Lett (2004)
35 R. R. Allison, G. H. Downie, R. Cuenca, X. H. Hu, C.J.H. Childs, C.H. Sibata, Photodiag. Photodyn. Therapy 1 27-42 (2004)
36 Chen W. and Zhang J., J. Nanosci. Nanotechnol. 6 1159-66 (2006)
37 F. Fabbri, F. Rossi, G. Attolini, G. Salviati, S. Iannotta, L. Aversa, R.
Verucchi, M. Nardi, N.Fukata, B. Dierre and Takashi Sekiguchi, Nanotechnology 21 345702 (2010)
38 Ethan D. Stenberg, David Dolphin, Tetrahedron 54 4151-4202 (1998)
39 Van Lier, J. E. in Photobiological Techniques, 216, 85-98 (1991)
40 V. Kral, J. Kralova, R. Kaplanek, t. Briza, P. Martasek, Physiol. Res.
55, S3-S26, (2006)
41 H.I. Adler, W.D. Fischer, A. Cohen, A.A. Hardigree Proc.Natl.Acad.Sci.USA 57:321-326 (1967)
Small magnetic nanoparticles (MNPs) in the super-paramagnetic state are suitable for both the diagnostic and the therapeutic approaches. In the field of diagnostics, they have been proposed as a contrast agent to enhance the magnetic resonance imaging (MRI) signal while in the field of therapeutics they can be used as magnetic vector in drug delivery and/or as heat mediators in hyperthermia treatment.
Hyperthermia properties and drug delivery are of particular interest. In order to be superparamagnetic the particles need to be small (diameter minor than 20 nm), but hyperthermia increase with the size.
The magnetic hyperthermia can be effective on cancer cells, as a consequence of their increased sensitivity to temperature higher than 41°C in comparison to healthy ones. Hyperthermia consists in the application of a magnetic radiofrequency field to the magnetic nanoparticles. The ability of a material to be a good hyperthermic mediator is measured by the specific absorption rate (SAR) that represents the thermic power developed by the MNPs per mass unit. In order to increase the efficiency of the hyperthermia treatment, the SAR value has to be maximized leading to a desired increment of temperature at low doses of MNPs and at lower frequencies and fields.
The actual work of scientific community for the achievement of this aim is being developed in three different ways: the choice of material, the optimization of the size and the change of shape. The choice of the material is driven by the requirements on the magnetic crystalline anisotropy, an intrinsic parameter tunable by composition and structure, which influences the hysteresis loop shape and consequently the SAR value. In MNPs, the maximization of hyperthermia effect is observed in proximity of the critical size for the super paramagnetic to the ferromagnetic transition. This value depends on the crystalline anisotropy: higher is the anisotropy value, smaller is the critical size.
At the same time, also the variation of the shape can produce an increase of the magnetic anisotropy by adding two non-negligible terms, the shape anisotropy directly related to the shape of MNPs and
the surface anisotropy, due to the dead layer of surface spins aligned perpendicular to the surface, which is influenced by the faceting of the MNPs.
Another factor that influence the hyperthermia is the nature of the NP stabilizers and coating. In the present chapter, I report the synthesis of magnetite nanoparticles obtained using different methods.
I tried different synthetic procedures in order to find the better result in term of homogeneous size distributions, crystal structure and ending functional groups in surfactants chains.
I started with the most famous procedure the co-precipitation (Massart’s procedure). This method started from a solution of iron (III) and iron (II) in stoichiometric ratio in basic condition, heated under mechanically stirrer. In literature there are thousands of articles that use this procedure. It’s an easy technique and requires mild conditions. The disadvantage is the formation of aggregate (A manuscript in preparation describe the interactions between nanoparticles obtained by co-precipitation and thermal decomposition method, “Lorentz microscopy sheds light on the role of dipolar interactions in magnetic hyperthermia” M. Campanini, R. Ciprian, E. Bedogni, V. Chiesi, A.
Mega, C. de Juliàn Fernàndez, F. Casoli, F. Rossi, E. Rotunno, V.
Grillo, F. Bigi, G. Salviati, and F. Albertini).
According to Massart’s procedure, magnetite nanoparticles were prepared and dried. Then, I tried to coat them with Au, to obtain core- shell nanoparticles where the shell could add a plasmonic effect and can easily functionalized with thiol-ending molecules.
Results and Discussions
I synthetized two samples: the first one was soluble in water phase and the second one in organic phase. The samples were studied by electron microscopy at IMEM-CNR.
This analysis (TEM images) shows the presence of stable nanoparticles (Figure 1, d, e, f pictures) with a large size distribution and a, b, c pictures show the presence of some aggregate and the absence of a core-shell structure. As reported in the literature, the method of co- precipitation leads to the formation of aggregates which even if
"covered" gold damage formation of aggregates in the aqueous phase.
Figure 1. TEM images of Au-Fe3O4 cluster water soluble (a, b, c) and Au-Fe3O4 organic soluble (d, e, f). TEM pictures show the broad size distribution in Au-Fe3O4 cluster organic soluble (images d, e, f). It is not easy understand if there are core-shell structures or if there are presence of both materials in a random distribution. Water soluble particles, as shown in the Figure 1a, 1b and 1c, are aggregate in big particles and cluster where it is easy see the presence of Fe3O4 and Au (like show in image HAADF: Z-contrast).
d# e# f#
With regard to the organic phase that is watched and the formation of particles stabilized but with a large dimensional range.
Then I tried the magnetite synthesis using microwave method in order to use also a different surfactant.
As described by Reimhult in 20111 nanoparticles were synthetized using a microwave loop, starting from a precursor of iron (III), Fe(ac)3,
and benzyalcohol as reducing agent-solvent in a flask, a lot of energy for few minutes. After that a solution of nitro-DOPA in DMF was added as stabilizer.
I did not obtain good results; indeed, as shown in the pictures, nanoparticles are immersed in a large amount of organic materials.
They have a narrow size distribution and the diameter of inorganic material is centered at 5 nm, is too small for our applications.
I also experimented the synthesis based on the thermal decomposition method. In literature there are many articles that describe this procedure for several applications. This methodology makes possible the use of different surfactants, opening the possibility to have different functional groups.
This type of synthesis starts from a precursor of iron (III) as Fe(acac)3
in presence of a reducing agent, surfactants and high boiling point solvent. Some of a preliminary experiments are reported below.
Figure 2. TEM pictures of nanoparticles obtained by a microwave method
I tried using phenyl ether as solvent, oleic acid and oleylamine as surfactants and tert-butylcathecol as reducing agent. The reaction was heated at 300°C for 30’.
I obtained magnetic nanoparticles in a large size distribution. TEM images (Figure 3).
The media diameter is 18 nm. There are many sizes and different shape. An usual shape was observed that looks like red blood cells.
These nanoparticles show the presence of monocrystalline structure like show in Figure 4, that correspond at Fe3O4 crystal structure.
Figure 3. TEM pictures of samples obtained by thermic decomposition
This picture shows a single nanoparticles with a single crystal structure, like shown in a diffraction patter. The results that we obtained were different from the results that Sun and Zang proposed in 2002, the explanation could be the different set up and different reducing reagents (the articles propose the use of 1,2-hexadecanediol).
In another experiment, I used phenyl ether as solvent, oleylamine as surfactant and ters-butylcathecol as reducing agent. The reaction was heated at 300°C for 30’. The nanoparticles obtained were stable and with a narrow size distribution and a media diameter centered around 9 nm. The negative aspect of this good sample was the difficulty to obtain a functional group easily to use to conjugate nanoparticle with other system.
I decided to follow a procedure reported in the literature to obtain nanoparticles of different sizes and stabilized by an organic shell that
could be modified successively. Good quality nanoparticles were obtained reacting Fe(acac)3 in the presence of 1, 2-hexadecanediol as reducing agent, oleic acid and oleylamine as surfactants and phenyl ether as solvent. 220 °C were reached for 30 minutes after a preheating at 200°
oleic acid oleylamine
O O O O
O O OO
O O OO
200°C, 30' 220°C, 30'
Figure 5. Synthetic approach for thermal decomposition method
Preheating was important in order to produce in situ an homogeneous precursor of iron to produce nanoparticles with a narrow size distribution.
As it is show in the picture of Figure 6 the nanoparticles were small and with a narrow dimension distribution, with a diameter centered at 3-4 nm. These types of nanoparticles are stable also after long time (months). For the good size distribution, high stability for long time and for good crystal structure we decided to study also the magnetic properties.
At IMEM-CNR the magnetic properties of these nanoparticles were examined.
Figure 6. TEM picture and dimension distribution of nanoparticles obtained by thermal decomposition (c)
Figure7. Magnetic study of NP-4 nm. It is in evidence that magnetization at highest field is 3.4± 0.3 /kg. This value is very low. Because of the small size, the particles are far from the saturation at room temperature.
The value of saturation magnetization was 3.4 Am2/Kg that was a low value but normal for magnetite nanoparticles with very small size.
In order to know the amount of magnetic material and organic part thermogravimetric analysis was performed. The total weight loss resulted to be 32%.
Figure 8. TGA analysis:The operative condition are air flux, Tstart= r.t., Tmax= 800°C, rate=10°/min. the total weight loss is 32%
The idea developed to bind the magnetite nanoparticles to the SiC/SiO2
nanowires, was the formation of a triazole ring between the two partners. This approach requires the introduction of complementary groups on the surface of the nanoparticles and of the nanowires, i.e.
terminal alkyne on NPs and azide groups on nanowires.
The introduction of alkyne groups was accomplished by ligand exchange procedure. Nanoparticles obtained by a previous step were dissolved in hexane solution in presence of 10-undecynoic acid. The reaction was heated. Nanoparticles were washed several times and the presence of alkyne group was studied by FT-IR analysis that show the stretching of C≡C at υ~2100 cm-1 and the stretching C≡C-H at υ~3210 cm-1.
# Figure 9. Undecynoic acid
Since the magnetic properties were unsatisfactory I increased the diameter of nanoparticles changing the thermal decomposition conditions. Dibenzyl ether was employed as solvent to reach highest temperature ~ 300 °C. After heating at 200 °C for 2 hours under nitrogen, the reaction was refluxed for 1 hour. These conditions give to particles more time to increase in dimension.
As shown in TEM images (Figure 10) nanoparticles have a narrow size distribution with a media diameter centred at 7 nm, and as reported in diffraction pattern the crystal structure matches with magnetite crystal structure. The magnetic characterisation was performed.
Figure 10. TEM images, diffraction patter, size distribution are shown in this figure. The first pictures show good homogeneous distribution, and a detail is shown in the last one. Diffraction patter shows magnetite crystal structure and the narrow size distribution is shown with a d= 7 nm.
Figure 11. Hysteresis loop at room temperature of 8 nm MNPs obtained by thermal decomposition and: left: maximum field of 1.5 T, right: maximum field of 0.2 T.
As you can see in the Figure 11, the nanoparticles reach the saturation around 60 Am2/kg and the zoom (right) shows the absence of hysteresis, evidencing that the nanoparticles have superparamagnetism properties and there is no-interaction between nanoparticles.
The nanoparticles synthetized in this way are stable and display a high magnetization value. Therefore it was also possible to study the hyperthermia properties.
As it is shown in Figure 12 nanoparticles, dispersed in hexane, increased the temperature of 4.2 K in 20 min if a frequency of 250 KHz and a magnetic field of 0.016 T were applied. This value showed the
possibility to use this type of nanoparticles for hyperthermia and urges us to search for increasing the particle dimensions.
Thanks to the collaboration with medical and veterinary groups, the biocompatibility of the synthesized nanoparticles was studied and the internalization was confirmed.
In literature there are many works dealing with the biocompatibility of magnetite nanoparticles. Indeed, the biocompatibility depends from the organic or inorganic shell around the nanoparticles and from their specific nature.2
The polarity of the organic shell can totally change also the mechanism of internalization. It also known that the shell should have both polar and apolar characteristics, since the nanoparticles have to pass through the cell wall (apolar) and have to stay inside the cytoplasm area (polar solution).
The internalization study was accomplished using A549 culture cells.
The nanoparticles sample was solubilized in DMSO (small amount) and after that diluted in water in order to decrease the concentration of DMSO (in high concentration this is toxic for cells).
The cells, after 24 hours (uptake time) were fixed in a resin using a protocol performed by Prof. Cacchioli and the resin-wafer was examined by TEM spectroscopy.
The nanoparticles were internalized inside the cells at intracytoplasmonic level, in cytoplasm area as shown in the following picture (Figure 14).
Biocompatibility of nanoparticles was studied evaluating the number of cells in life and death cells at different concentrations.
Figure 14. TEM image (obtained at 80 MeV) show the presence of nanoparticles inside the cytoplasm area.
0 1 10 25 50 100
0 200 400 600 800
n° cells (x103)
0 1 10 25 50 100
0 10 20 30 40 50
cell death (%)
Figure 15. Histograms show that there isn’t inhibition of proliferation and absence of cell death also for high nanoparticles concentration.
The histograms reported in Figure 15 show that no inhibited proliferation and cell death is found. Apoptosis evaluation was done by Trypan Blue Test (Figure 16) that evidenced the absence of apoptosis.
This study bring to light that the prepared nanoparticles can be incorporated inside the cells (the study was performed only in A549, cancer cells) and are biocompatible. Therefore they can be anchored to biocompatible nanowires.
Very recently I obtained preliminary experiments promising results from nanoparticles with a cubic shape obtained by thermal decomposition. The synthesis started from the same reagents previously employed, i.e. Fe(acac)3, 1, 2-hexadecanediol, oleic acid, oleylamine, and benzyl ethers. The temperature was increased at a heating rate of 7
°C/min up to 300 °C and maintained for 1 h. Some procedures are reported in the literature to obtain a cubic form, but they are not easy to reproduce, since the heating conditions are crucial. Small changes in the temperature values and also in the heating rate determine shape and dimension variation.3 TEM images show the size of particles, that was
0 10 20 30 40 50
cell death (% PI positive cells)
Figure 16 Trypan test shows the absence of apoptosis (cell in life are in blue and dead cells are in red).
Histogram shows the absence of apoptosis by cells count. !